Microbuckling Instability and the Second Yield during the Deformation of Semicrystalline Polyethylene

Deformation instabilities, such as microbuckling or lamellar fragmentation due to slip localization, play a very important role in the deformation of semicrystalline polymers, although it still not well explored. Such instabilities often appear necessary to modify the deformation path and facilitate strain accommodation in an energy-minimizing manner. In this work, microbuckling instability was investigated using partially oriented, injection-molded (IM) samples of high-density polyethylene, deformed by a plane-strain compression. Deformed samples were probed by SEM, X-ray (small- and wide-angle X-ray scattering: SAXS, WAXS), and differential scanning calorimetry (DSC). It was found that microbuckling instability, followed quickly by the formation of lamellar kinks, occurred in high-density polyethylene (HDPE) at a true strain of about e = 0.3–0.4, mainly in those lamellar stacks which were initially oriented parallel to the compression direction. This phenomenon was observed with scanning electron microscopy, especially in the oriented skin layers of IM specimens, where a chevron morphology resulting from lamellae microbuckling/kinking was evidenced. Macroscopically, this instability manifested as the so-called “second macroscopic yield” in the form of a hump in the true stress–true strain curve. Microbuckling instability can have a profound effect on the subsequent stages of the deformation process, as well as the resulting structure. This is particularly important in deforming well-oriented lamellar structures—e.g., in drawing pre-oriented films of a semicrystalline polymer, a process commonly used in many technologies.


Introduction
Semicrystalline polymers demonstrate a high ability to deform plastically, which appears to be one of their most essential properties, and has therefore been extensively studied (see reviews-e.g., [1][2][3][4]). The deformability of semicrystalline polymers can largely be attributed to their unique morphology, which at a basic level consists of thin alternating crystalline and amorphous layers, tightly linked together by chains crossing the interface. At temperatures above the glass transition, the rubber-like amorphous layers appear very soft and compliant compared to the crystalline layers; nevertheless, both components must deform cooperatively to satisfy the material integrity condition [4]. The deformation of a semicrystalline polymer turns out to be a complex process, involving various mechanisms active at different stages. The crystalline lamellae are principally deformed by crystallographic mechanisms [1][2][3][4][5], such as crystallographic slip (which is the dominant mechanism), twinning, or martensitic transformation. The non-crystallographic mechanism-strain-induced "melting-recrystallization" transition-has also been suggested by some where h o denotes the initial height of the specimen, ∆h is the measured displacement of the plunger, and h = h o − ∆h is actual specimen height, while λ = CR = h o /h is the compression ratio. As the area of the sample under load in a channel-die remains constant (equal to the cross-section of the plunger) the true stress can be calculated with the following simple formula: where F is the measured force and A is the surface area of the plunger.
The coordinate system used throughout this paper is related to the geometry of the channel-die: the loading direction (LD) is the direction of the compressive force applied to the plunger; the constraint direction (CD) is perpendicular to the sidewalls of the channel; and the flow direction (FD) is parallel to the channel length-i.e., directed towards its opening. In most of the experiments, the LD coincided where ∆h f is the heat of the melting of the sample determined from the DSC melting curve and ∆h f100 = 293 J/g is the heat of the melting of 100% crystalline PE [37].

Results and Discussion
Rectangular bar samples of HDPE were produced by injection molding (IM). Micrographs of the cross-section of the IM bar perpendicular to the injection direction revealed the core-skin morphology; an opaque core about 2 mm in thickness was surrounded by an almost transparent skin layer, about 1 mm thick-cf. Figure 1a. The IM bars demonstrated some shrinkage upon cooling, and therefore had to be carefully machined to obtain specimens with a regular parallelepiped shape that would fit very precisely into the channel of the channel-die compression fixture. The method is illustrated in Figure 1b. As a result, rectangular bars were prepared for deformation tests, with a cross-section of 8 × 3.85 mm 2 . The morphology of the bars obtained then consisted of a flat core . On a black background, the opaque core layer looks light, and the transparent skin layer looks dark; (b) schematic drawing illustrating how specimens were cut from IM bars; (c) 2D-WAXS and 2D-SAXS images obtained in transmission, separately for the skin layer and the core layer, when the sample was illuminated along the normal direction (n.d.) or the transverse direction (t.d.).
To examine the structure and morphology of the layers, small samples approximately 1 mm thick were taken from either the skin or the core layers of the IM bar and then examined with DSC, X-ray (both 2D-SAXS and 2D-WAXS), and scanning electron microscopy. The DSC melting data revealed that the skin layers contain crystals that melt at a slightly lower temperature than those in the core layer (134.7 vs. 135.4 °C ), which implies that crystallites in the skin layers are only slightly thinner than in the core layer. The crystallinity of both layers is nearly the same: the values of Xc = 64.3 wt.% and Xc = 63.9 wt.% were estimated for the skin layer and the core layer, respectively. The results of X-ray scattering investigations are shown in Figure 1c. The SAXS images of the skin layer, when it was illuminated with X-ray along either n.d. or t.d., show a sharp two-point pattern that suggests a well-oriented lamellar structure with a lamella normal oriented preferentially along the injection direction, i.d. This finding is supported by 2D-WAXS images of the skin layer, where the observed position of the (110) and (200) reflections near t.d. can suggest the preferred orientation of the chain axis close to i.d.-i.e., similar to the preferred orientation of the lamella normal. The 2D-WAXS patterns of the skin layer ( Figure 1) show relatively broad diffraction arcs of (110) plane centered along t.d., and (200) arcs also centered along t.d. Additionally, a second pair of (200) arcs was observed along i.d, although they were weaker than those observed along t.d. Such a diffraction pattern may suggest a crystalline texture consisting of two components. The main, stronger . On a black background, the opaque core layer looks light, and the transparent skin layer looks dark; (b) schematic drawing illustrating how specimens were cut from IM bars; (c) 2D-WAXS and 2D-SAXS images obtained in transmission, separately for the skin layer and the core layer, when the sample was illuminated along the normal direction (n.d.) or the transverse direction (t.d.).
To examine the structure and morphology of the layers, small samples approximately 1 mm thick were taken from either the skin or the core layers of the IM bar and then examined with DSC, X-ray (both 2D-SAXS and 2D-WAXS), and scanning electron microscopy. The DSC melting data revealed that the skin layers contain crystals that melt at a slightly lower temperature than those in the core layer (134.7 vs. 135.4 • C), which implies that crystallites in the skin layers are only slightly thinner than in the core layer. The crystallinity of both layers is nearly the same: the values of X c = 64.3 wt.% and X c = 63.9 wt.% were estimated for the skin layer and the core layer, respectively. The results of X-ray scattering investigations are shown in Figure 1c. The SAXS images of the skin layer, when it was illuminated with X-ray along either n.d. or t.d., show a sharp two-point pattern that suggests a well-oriented lamellar structure with a lamella normal oriented preferentially along the injection direction, i.d. This finding is supported by 2D-WAXS images of the skin layer, where the observed position of the (110) and (200) reflections near t.d. can suggest the preferred orientation of the chain axis close to i.d.-i.e., similar to the preferred orientation of the lamella normal. The 2D-WAXS patterns of the skin layer ( Figure 1) show relatively broad diffraction arcs of (110) plane centered along t.d., and (200) arcs also centered along t.d. Additionally, a second pair of (200) arcs was observed along i.d, Polymers 2020, 12, 2208 7 of 18 although they were weaker than those observed along t.d. Such a diffraction pattern may suggest a crystalline texture consisting of two components. The main, stronger component consists of crystals preferentially oriented with poles of (110) and (200) planes perpendicular to i.d., which implies the chain axis close to i.d., just like the lamella normal. This is probably due to a structure formed under strong flow conditions, referred to as the "Keller/Machin II" mode, where the lamellae are flat and the c-axis remains parallel to the injection direction [38,39]. The second, clearly weaker texture component, manifested by the broadening of the (110) arc and the diffraction arc of (200) centered along i.d., was probably produced by lamellae grown in the form of twisted ribbons, resulting in the rotation of the crystallographic a-and c-axis around the b-axis. This structure is termed the "Keller/Machin I" mode, and is usually formed at weaker flow [39]-here, in the IM samples, possibly at the boundary of the skin layer just next to the core layer. In contrast to the skin layer, the core exhibited a uniform SAXS ring when illuminated along t.d., and an almost uniform scattering ring seen in the n.d.-view, with only a slightly higher scattering intensity along i.d. than along t.d. (cf. Figure 1c). At the same time, the corresponding 2D-WAXS images also show almost uniform diffraction rings, corresponding to the (110) and (200) planes of the orthorhombic unit cell of PE. All these features indicate an almost random orientation of the lamellae in the core layer, with only a trace of the preferred orientation perpendicular to i.d. The above-postulated preferred orientation of lamellae in the skin and core layers was confirmed by direct microscopical observations using a scanning electron microscope (SEM). Figure 2a,b present representative SEM micrographs of the skin and core layers, respectively. It can be easily seen in Figure 2a that virtually all the lamellae in the skin layer are flat and well-oriented perpendicular to i.d., while the micrograph in Figure 2b suggests no apparent preferred orientation of lamellae in the core layer. The lamellae in the skin layer seem to be relatively short compared to the core layer or fragmented, although it cannot be ruled out that this appearance of lamella in the micrograph is merely an artifact resulting from some overetching that may have occurred during sample preparation, particularly along the concentrations of dislocation lines or at sites of greater concentration of other defects that may give the impression of disrupted lamellae [31]. The lamellae in the core layer are long and appear to be organized in higher-order structures, such as spherulites (which can be recognized at a lower magnification), which are large enough to scatter visible light and thus make the core layer opaque. In contrast, the well-ordered skin layer (lacking higher-order morphological structures) does not scatter light so much, rendering it almost transparent.
Polymers 2020, 12, x FOR PEER REVIEW 7 of 19 component consists of crystals preferentially oriented with poles of (110) and (200) planes perpendicular to i.d., which implies the chain axis close to i.d., just like the lamella normal. This is probably due to a structure formed under strong flow conditions, referred to as the "Keller/Machin II″ mode, where the lamellae are flat and the c-axis remains parallel to the injection direction [38,39]. The second, clearly weaker texture component, manifested by the broadening of the (110) arc and the diffraction arc of (200) centered along i.d., was probably produced by lamellae grown in the form of twisted ribbons, resulting in the rotation of the crystallographic a-and c-axis around the b-axis. This structure is termed the "Keller/Machin I″ mode, and is usually formed at weaker flow [39]-here, in the IM samples, possibly at the boundary of the skin layer just next to the core layer. In contrast to the skin layer, the core exhibited a uniform SAXS ring when illuminated along t.d., and an almost uniform scattering ring seen in the n.d.-view, with only a slightly higher scattering intensity along i.d. than along t.d. (cf. Figure 1c). At the same time, the corresponding 2D-WAXS images also show almost uniform diffraction rings, corresponding to the (110) and (200) planes of the orthorhombic unit cell of PE. All these features indicate an almost random orientation of the lamellae in the core layer, with only a trace of the preferred orientation perpendicular to i.d. The above-postulated preferred orientation of lamellae in the skin and core layers was confirmed by direct microscopical observations using a scanning electron microscope (SEM). Figure 2a,b present representative SEM micrographs of the skin and core layers, respectively. It can be easily seen in Figure 2a that virtually all the lamellae in the skin layer are flat and well-oriented perpendicular to i.d., while the micrograph in Figure 2b suggests no apparent preferred orientation of lamellae in the core layer. The lamellae in the skin layer seem to be relatively short compared to the core layer or fragmented, although it cannot be ruled out that this appearance of lamella in the micrograph is merely an artifact resulting from some overetching that may have occurred during sample preparation, particularly along the concentrations of dislocation lines or at sites of greater concentration of other defects that may give the impression of disrupted lamellae [31]. The lamellae in the core layer are long and appear to be organized in higher-order structures, such as spherulites (which can be recognized at a lower magnification), which are large enough to scatter visible light and thus make the core layer opaque. In contrast, the well-ordered skin layer (lacking higher-order morphological structures) does not scatter light so much, rendering it almost transparent.  The observation plane normal to n.d. was exposed by microtoming, followed by chemical (permanganic) etching to reveal details of the lamellar structure.
Polymers 2020, 12, 2208 8 of 18 The samples machined out from IM bars and having a well-defined three-layer sandwich morphology seemed very useful for investigating some aspects of the plastic deformation of a semicrystalline polymer, in particular the buckling instability [9][10][11][13][14][15]. Since both the skin and core layers are thick (approx. 1 and 2 mm, respectively) and separated by a thin transition layer, their deformation behavior can be considered almost independent of each other and can be assessed separately in a single compression experiment. The oriented (skin) and unoriented (core) components operate in parallel when the sample is loaded in any direction along the layering, while they act in series when it is loaded along the n.d., perpendicular to the layers. Figure 3 shows the mechanical response of IM sandwich-like samples when subjected to plane-strain compression, compared to a non-oriented, uniform CM sample (obtained by compression molding) deformed under the same conditions. The CM sample exhibited a spherulitic morphology similar to that observed in the core of the IM sample, with no trace of preferred lamellar orientation. The deformation of the CM sample and the underlying mechanisms were studied in detail and reported in our recent papers [10,11]. The main plot in Figure 3 shows the enlarged initial part of the true stress-true strain curves, while the inset shows the same curves over the full range of stress and strain. In two independent experiments, IM samples were loaded in two orthogonal directions parallel to the sample skin-core layering, either along the transverse direction or along the injection direction: LD = t.d. or LD = i.d., respectively. These correspond to the LD parallel or perpendicular to the plane of the preferred orientation of lamellae in the skin layer, respectively. Additionally, the sample compressed along the n.d. was also tested (LD was then perpendicular to the skin and core layers, as well as to the lamella normal in the skin layer). The samples machined out from IM bars and having a well-defined three-layer sandwich morphology seemed very useful for investigating some aspects of the plastic deformation of a semicrystalline polymer, in particular the buckling instability [9][10][11][13][14][15]. Since both the skin and core layers are thick (approx. 1 and 2 mm, respectively) and separated by a thin transition layer, their deformation behavior can be considered almost independent of each other and can be assessed separately in a single compression experiment. The oriented (skin) and unoriented (core) components operate in parallel when the sample is loaded in any direction along the layering, while they act in series when it is loaded along the n.d., perpendicular to the layers. Figure 3 shows the mechanical response of IM sandwich-like samples when subjected to plane-strain compression, compared to a non-oriented, uniform CM sample (obtained by compression molding) deformed under the same conditions. The CM sample exhibited a spherulitic morphology similar to that observed in the core of the IM sample, with no trace of preferred lamellar orientation. The deformation of the CM sample and the underlying mechanisms were studied in detail and reported in our recent papers [10,11]. The main plot in Figure 3 shows the enlarged initial part of the true stress-true strain curves, while the inset shows the same curves over the full range of stress and strain. In two independent experiments, IM samples were loaded in two orthogonal directions parallel to the sample skin-core layering, either along the transverse direction or along the injection direction: LD = t.d. or LD = i.d., respectively. These correspond to the LD parallel or perpendicular to the plane of the preferred orientation of lamellae in the skin layer, respectively. Additionally, the sample compressed along the n.d. was also tested (LD was then perpendicular to the skin and core layers, as well as to the lamella normal in the skin layer).  began to flow with a slowly increasing stress, which, however, remained all the time lower than that in CM. In contrast, the true stress observed in the IM (LD = t.d.) sample after passing the yield point continued to increase with the strain slightly faster than in CM and exceeded the stress observed in the CM sample at the true strain of e ≈ 0.2. The stress in IM (LD = t.d.) sample then remained higher than in the CM sample up to the highest strains. In the strain-hardening range, the slightly different slopes of the curves of the IM and CM samples ultimately led to a noticeable difference in the stress arising at the highest strains, approaching e = 2.0; the IM (LD = i.d.) (compressed perpendicularly to the preferred orientation plane of lamellae in the skin layers-i.e., along the preferred direction of the chain) demonstrated a lower strain hardening rate and consequently lower ultimate stress than CM, while the IM (LD = t.d.) sample-i.e., that compressed parallel to the preferred lamellar plane in the skin layer-exhibited a stronger strain-hardening effect than CM. The sample loaded along the n.d., (perpendicular to the skin core layering) demonstrated a stress-strain curve similar to that of the CM sample.
An important feature can be observed on the true stress-true strain curves shortly after passing the yield point, in the true strain range of about e = 0.3. It is a low and broad hump observed in the stress-strain curves of the CM, IM (LD = t.d.), and possibly IM (LD = n.d.) samples. Interestingly, such a hump cannot be discerned on the curve of the IM (LD = i.d.) sample. This hump is better developed and centered at the slightly smaller strain in the IM sample (LD = t.d.) than in the CM unoriented material-e ≈ 0.30 vs. 0.33. A very small hump is barely discernible on the curve of the IM (LD = n.d.) sample at a similar position to that seen in CM. A characteristic bulge similar to the hump discussed here was frequently observed in the stress-strain curves of various semicrystalline polymers shortly after passing the yield point, and was commonly referred to as the second yield [40][41][42][43]. This was often associated with the activation of a heterogeneous/coarse chain slip (block slip) [43][44][45][46][47] or with the activation of slip transverse to the chain direction [48]. In our recent works [10,11,15], we have postulated that the second yield point is rather associated with a certain deformation instability in the form of the microbuckling of lamellae followed by their kinking. This instability is experienced by stacks of lamellae, which at the beginning were specifically oriented parallel to the direction of compression (alternatively, in tensile deformation, by lamellae that were oriented perpendicular to the direction of drawing). Microbuckling, beginning as an elastic instability [16], leads to undulations of the lamellae that quickly turn into the formation of angular kinks, which involves irreversible plastic deformation and/or limited damage, especially in hinges of the sharp kink profiles [4,11,16,20,21]. The formation of such kinks is extremely important for the subsequent deformation behavior of the material, especially in some oriented structures, because kinking induces a quick and practically irreversible rotation of these lamellae, which were oriented initially parallel to the load and then underwent microbuckling, such as those in the polar region of spherulites or in oriented skin layers of the IM sample (when compressed perpendicularly to i.d.). Prior to buckling, these lamellae were not able to deform by any crystallographic mechanism due to too low resolved shear stress in the plane and direction of the potential slip system. The only deformation mechanism available for a stack of such lamellae was the so-called lamella separation, consisting of the dilatation of the interlamellar soft amorphous layer in the direction of their thickness, yet this mechanism was strongly constrained due to the very low compressibility of the rubber-like amorphous phase (a Poisson ratio close to ν = 1 /2, a very high bulk modulus K), the large lateral sizes of the amorphous and crystalline layers, and the very strong coupling between layers; the interlamellar layer of such an almost incompressible amorphous material tends to contract laterally (in the plane of the layer) when stretched along its thickness to maintain a constant volume, however this contraction is severely restricted due to the large lateral dimensions of the layer compared to the thickness, and the very strong connectivity of the amorphous layer with the adjacent crystalline layers. These constraints are very effective in limiting lateral contraction and thus in "locking" this dilatational mode of deformation. This effect can also be explained in terms of high oedometric modulus, which can be expressed by: For a rubber-like amorphous polymer, ν is close to 1 /2, hence E oed ≈ 2K-i.e., it appears very high, a few orders of magnitude higher than Young's modulus E. A high value of the oedometric modulus E oed implies a very limited dilatation of the amorphous layers in response to tensile stress along the thickness direction-i.e., "locking" the lamella separation mechanism. As a consequence, the entire deformation process was temporarily locked locally with growing stresses, which would soon inevitably lead to deformation instability. To alleviate high lateral stress, the layered material may respond either with cavitation in the amorphous layers or with cooperative buckling of the crystalline/amorphous layers, possibly followed by their kinking and the formation of a chevron morphology. The particular response depends on the material properties and the stress field (tension/compression), but the microbuckling of layers often wins that competition, especially in the compression modes of deformation that usually suppress cavitation. The change in the orientation of lamellae, which occurred in the folds or kinks initiated by microbuckling instability, causes an increase in the resolved shear stress for the potential crystallographic slip system in these lamellae. This increase may appear to be sufficient to activate that slip mechanism. Moreover, kinking causes a collapse of the rigid lamellar structure, which may further relieve the lamellae of some of the previous morphological constraints. All these phenomena unlock the deformation process in these areas by opening up a new route for the easy plastic deformation of the crystalline lamellae-those reoriented rapidly in kink limbs can now deform relatively easily due to crystallographic slip, like other lamellae that had already been oriented favorably to such slip. This change allows the strain to be accommodated more easily and prevents excessive stress build-up, thus allowing further plastic deformation without the premature failure of the material.
It was established that the microbuckling is driven by significantly different levels of stiffness of the hard (crystalline) and soft (amorphous) layers and their strong interfacial connectivity through numerous tie-molecules and entangled loops [9,12,13,16]. It was found that it depends primarily on the ratio of stiffness of the layers and the concentration of the so-called stress transmitters at the crystal-amorphous interface (like tie-molecules, entangled loops, etc.) [10,11]. The stiffness of the layers, in turn, is determined by their thickness and the modulus of elasticity of the respective phase.
The microbuckling/kinking instability, which can facilitate the activation of new deformation mechanisms of lower plastic resistance, is often revealed in the stress-strain curve as a characteristic hump or bulge, which is commonly called the second macroscopic yield. We reported in our previous papers [10,11,15] a hump in the form of a very low and broad maximum related to the second yield in unoriented samples of several grades of polyethylene, which was observed around e ≈ 0.3-0.4. Concurrently, a rapid reduction in the scattering intensity in FD was noticed in the 2D-SAXS images in the same strain range. The scattering in FD is due to lamellar stacks that are oriented with the lamella planes parallel to LD (lamella normal parallel to FD). A sharp decrease in this component of scattering indicated the effective removal of such a specific orientation of lamellae with advancing strain. Moreover, the four-point pattern began to develop in the 2D-SAXS images (CD-view) shortly thereafter, at e ≥ 0.4, which revealed two emerging populations of lamellae, both inclined symmetrically to the direction of plastic flow and giving rise to chevron morphology. All these phenomena illustrated the same deformation mechanism, which in our opinion was the microbuckling instability that was quickly followed by the formation of lamellar kinks, activated at approx. e ≈ 0.3-0.4.
Similar observations were made for the samples studied in this work. First, we can note that an already reported hump in the stress-strain curves indicating the second macroscopic yield is larger in the IM (LD = t.d.) sample than in the CM sample, possibly because the population of lamella initially oriented parallel to LD in the IM (LD = t.d.) sample (including the skin layers where nearly all the lamellae were oriented in this way) is significantly larger than in the CM sample. The same large fraction of lamellae oriented parallel to LD can be found in the IM (LD = n.d.) sample, yet the core and skin layers here act in series upon load, as opposed to IM (LD = t.d.), where they operate in parallel. Consequently, the contribution of the oriented layers to the second yield in the IM (LD = t.d.) sample is greater than that in the IM (LD = n.d.) or CM. In contrast, the lamellae in the skin layer of the IM (LD = i.d.) sample are oriented perpendicular to LD, and thus the population of lamellae parallel to LD, which might contribute to microbuckling and kinking, is highly reduced compared to the IM (LD = t.d.) or even to the CM sample. Consequently, the IM (LD = i.d.) sample practically does not show a hump of the second yield in the true stress-true strain curve.
In a separate experiment, IM samples were deformed to different, pre-selected strains. After the deformation to the desired strain, small specimens were cut from the skin and core layers of the deformed sample and examined with X-rays. Figure 4 shows a series of 2D-SAXS images in the CD-view (illumination of the sample with X-rays parallel to CD) of samples taken from the skin and the core layer of deformed IM samples (LD = t.d.). For comparison, images of CM samples deformed under analogous conditions are presented. In both series of images obtained for IM samples, one can observe an evolution of the X-ray pattern from an initial two-arc (core) or two-point (skin) pattern to the four-point pattern, which can be recognized at a strain of around e ≈ 0.4-0.5 and is fully developed above e = 0.7. Such a four-point pattern suggests the appearance of two populations of lamellae oriented symmetrically to the FD and contributing to the chevron morphology, which may be due to the lamella microbuckling and kinking. At e ≥ 1.0, the scattering images of the core and skin parts of the sample become very similar to each other and further change with the strain in a very similar fashion, indicating that the active deformation mechanism is identical for both the skin and the core parts of the sample. To illustrate this, the last row of Figure 4 shows SAXS images of the skin and core parts of the same sample deformed to e = 1.75, which are indeed very similar. The full sequence of the evolution of the SAXS pattern with increasing strain, including the e = 1.0-2.0 range not shown here, obtained for similar HDPE samples is presented in [10,11]. It has already been found that the main deformation mechanism at e ≥ 1.0 is an intense crystallographic slip in the direction parallel to the chain direction, which is already well advanced and therefore prone to a loss of stability and thus to localization. Such instability leads to lamellae fragmentation and then to a restructuring of the resultant blocks (a transformation known in tensile deformation as fibrillation), leading to high ordering and the formation of a new long period along the direction of plastic flow [10,11,49]. Figure 5 shows the azimuth profiles determined from the 2D images presented in Figure 4 in the range of the scattering vector around the value corresponding to the maximum intensity. These profiles demonstrate that the four-point pattern can be distinguished already at e = 0.3 in the core part of the sample-the maximum observed initially along FD splits into two separate peaks-and at e ≈ 0.4 in the skin layer (the maximum along FD broadens significantly and lowers; its shape clearly suggests two overlapping peaks). At the same time, a sharp drop in the scattering intensity measured along FD in the strain range of e ≈ 0.3-0.5 can be discerned, both in the core and skin parts of the sample, as illustrated in Figure 5. Figure 6 presents the 2D-WAXS patterns (CD-view) obtained for the same set of the deformed IM samples (LD = t.d.), already characterized by SAXS. It can be seen that the (110) and (200) planes, both parallel to the chain direction in the crystal lattice, are initially oriented preferentially close to LD (t.d.); the arcs of the high diffraction intensity of (110) and (200) planes can be found near the equator-marked with arrows in Figure 6-which suggests that the preferred orientation of the chain direction parallel to FD = i.d., as expected. As the strain increases, the maximum diffraction intensity of both planes (110) and (200) jumps to a new position, at some angle from t.d., which can be easily observed in the images of the sample core. This indicates the rotation of the chain axis away from the flow direction (FD = i.d.), which is consistent with the rapid rotation of lamellae detected by SAXS, all of which could have been expected for lamellae kinking. At higher strains, e > 1.0, the activity of the chain slip brings the strong orientation of the chain axis along FD (hence, the maxima of diffraction intensity of (110) and (200) planes are observed near LD-i.e., perpendicular to FD).     Figure 7 presents 2D-SAXS images and Figure 9 2D-WAXS images, all obtained under X-ray illumination along CD (CD-view). Figure 8 shows the azimuth scans obtained from the SAXS images of Figure 7 (integrated within the range of the scattering vector around the value corresponding to the maximum intensity). It can be seen from Figs 7 and 8 that the intensity of scattering along the FD, and therefore the population of the lamellae oriented perpendicular to FD (parallel to LD), is slightly reduced in the      Figure 7 presents 2D-SAXS images and Figure 9 2D-WAXS images, all obtained under X-ray illumination along CD (CD-view). Figure 8 shows the azimuth scans obtained from the SAXS images of Figure 7 (integrated within the range of the scattering vector around the value corresponding to the maximum intensity). It can be seen from Figs 7 and 8 that the intensity of scattering along the FD, and therefore the population of the lamellae oriented perpendicular to FD (parallel to LD), is slightly reduced in the       Figure 7 presents 2D-SAXS images and Figure 9 2D-WAXS images, all obtained under X-ray illumination along CD (CD-view). Figure 8 shows the azimuth scans obtained from the SAXS images of Figure 7 (integrated within the range of the scattering vector around the value corresponding to the maximum intensity). It can be seen from Figs 7 and 8 that the intensity of scattering along the FD, and therefore the population of the lamellae oriented perpendicular to FD (parallel to LD), is slightly reduced in the   Figure 7 presents 2D-SAXS images and Figure 9 2D-WAXS images, all obtained under X-ray illumination along CD (CD-view). Figure 8 shows the azimuth scans obtained from the SAXS images of Figure 7 (integrated within the range of the scattering vector around the value corresponding to the maximum intensity). It can be seen from Figures 7 and 8 that the intensity of scattering along the FD, and therefore the population of the lamellae oriented perpendicular to FD (parallel to LD), is slightly reduced in the core part and is very small, almost absent, in the skin layer of the initial sample prior to deformation. Accordingly, the formation of the four-point pattern is observed upon deformation only in the core (e ≥ 0.3), while the skin shows practically no such signature in the SAXS pattern. There is only a reduction in height and a slight broadening of the peak centered at LD, which can be observed at e = 0.3-0.5. Instead of a four-point pattern, a new long period begins to emerge along FD at e ≈ 0.7, which can be read as a mark of extensive lamellae fragmentation and restructuring [10,11,49,50]. These observations are easy to understand, because for the LD = i.d. geometry, the relatively poorly oriented core layer does not differ significantly in lamellar orientation from the core of the IM (LD = t.d.) sample, as described earlier. Consequently, in the IM (LD = i.d.) sample, there are still enough lamellae oriented parallel to LD to respond to deformation with microbuckling and kinking, similarly to the case of samples with LD = t.d. On the other hand, the highly oriented skin layer of the IM (LD = i.d.) sample contains virtually no lamellae parallel to LD that are prone to microbuckling, which would lead to a four-point SAXS pattern. Most of the lamellae here are oriented perpendicular to LD, which makes them more vulnerable to cleavage and fragmentation under load. As a result, a new long period along the FD appears earlier in the SAXS pattern of the skin layer, instead of the four-point feature. The evolution of the crystal orientation revealed in the 2D-WAXS images presented in Figure 9 confirms that picture-there is a jump in the orientation of the chain direction (inferred from the rotation of (hk0) planes) in the core layer already at a low deformation, which is presumably related to the formation of lamellar kinks. On the other hand, the orientation of crystallites in the skin layer begins to change slowly at low strains and then faster at e ≈ 0.5, which is probably related to the progression of crystallographic slip and lamella fragmentation phenomena. These mechanisms ultimately led to the final well-oriented crystalline texture observed at high strain above e = 1.75 in both the skin and core layers. core part and is very small, almost absent, in the skin layer of the initial sample prior to deformation. Accordingly, the formation of the four-point pattern is observed upon deformation only in the core (e ≥ 0.3), while the skin shows practically no such signature in the SAXS pattern. There is only a reduction in height and a slight broadening of the peak centered at LD, which can be observed at e = 0.3-0.5. Instead of a four-point pattern, a new long period begins to emerge along FD at e  0.7, which can be read as a mark of extensive lamellae fragmentation and restructuring [10,11,49,50]. These observations are easy to understand, because for the LD = i.d. geometry, the relatively poorly oriented core layer does not differ significantly in lamellar orientation from the core of the IM (LD = t.d.) sample, as described earlier. Consequently, in the IM (LD = i.d.) sample, there are still enough lamellae oriented parallel to LD to respond to deformation with microbuckling and kinking, similarly to the case of samples with LD = t.d. On the other hand, the highly oriented skin layer of the IM (LD = i.d.) sample contains virtually no lamellae parallel to LD that are prone to microbuckling, which would lead to a four-point SAXS pattern. Most of the lamellae here are oriented perpendicular to LD, which makes them more vulnerable to cleavage and fragmentation under load. As a result, a new long period along the FD appears earlier in the SAXS pattern of the skin layer, instead of the fourpoint feature. The evolution of the crystal orientation revealed in the 2D-WAXS images presented in Figure 9 confirms that picture-there is a jump in the orientation of the chain direction (inferred from the rotation of (hk0) planes) in the core layer already at a low deformation, which is presumably related to the formation of lamellar kinks. On the other hand, the orientation of crystallites in the skin layer begins to change slowly at low strains and then faster at e  0.5, which is probably related to the progression of crystallographic slip and lamella fragmentation phenomena. These mechanisms ultimately led to the final well-oriented crystalline texture observed at high strain above e = 1.75 in both the skin and core layers.   core part and is very small, almost absent, in the skin layer of the initial sample prior to deformation. Accordingly, the formation of the four-point pattern is observed upon deformation only in the core (e ≥ 0.3), while the skin shows practically no such signature in the SAXS pattern. There is only a reduction in height and a slight broadening of the peak centered at LD, which can be observed at e = 0.3-0.5. Instead of a four-point pattern, a new long period begins to emerge along FD at e  0.7, which can be read as a mark of extensive lamellae fragmentation and restructuring [10,11,49,50]. These observations are easy to understand, because for the LD = i.d. geometry, the relatively poorly oriented core layer does not differ significantly in lamellar orientation from the core of the IM (LD = t.d.) sample, as described earlier. Consequently, in the IM (LD = i.d.) sample, there are still enough lamellae oriented parallel to LD to respond to deformation with microbuckling and kinking, similarly to the case of samples with LD = t.d. On the other hand, the highly oriented skin layer of the IM (LD = i.d.) sample contains virtually no lamellae parallel to LD that are prone to microbuckling, which would lead to a four-point SAXS pattern. Most of the lamellae here are oriented perpendicular to LD, which makes them more vulnerable to cleavage and fragmentation under load. As a result, a new long period along the FD appears earlier in the SAXS pattern of the skin layer, instead of the fourpoint feature. The evolution of the crystal orientation revealed in the 2D-WAXS images presented in Figure 9 confirms that picture-there is a jump in the orientation of the chain direction (inferred from the rotation of (hk0) planes) in the core layer already at a low deformation, which is presumably related to the formation of lamellar kinks. On the other hand, the orientation of crystallites in the skin layer begins to change slowly at low strains and then faster at e  0.5, which is probably related to the progression of crystallographic slip and lamella fragmentation phenomena. These mechanisms ultimately led to the final well-oriented crystalline texture observed at high strain above e = 1.75 in both the skin and core layers.   As discussed above, the mechanical and X-ray scattering data, presented in our previous papers [10,11,15] as well as in this article, strongly support the hypothesis of deformation instability in the form of the microbuckling of lamellae, followed by their kinking and the local formation of a chevron morphology. The microbuckling instability leading to sinusoidal undulations of the lamellae is initially elastic [16], but the subsequent formation of kinks entails some plastic deformation and possibly damage phenomena around the hinge of the kink [11,21]. This manifests itself macroscopically in the stress-strain curve in the form of a hump, commonly referred to as the second macroscopic yield, as the microbuckling helps to overcome the temporary barrier to further deformation and allows the relatively easy plastic deformation to continue, facilitating new deformation mechanisms in the just-kinked lamellae-such as crystallographic slips, previously inaccessible to these lamellae before buckling. However, to obtain the direct evidence of such postulated behavior of the material during its deformation, microscopic observations of deformed samples that could confirm conclusions drawn from the X-ray data seemed highly desirable. Therefore, the microscopic observations of samples deformed to various strains were carried out using a scanning electron microscope (SEM). Both the skin and core of the sample were examined in the CD-view (LD-FD observation plane). The LD-FD plane of observation was first exposed by microtoming, and then the lamellar morphology in this plane was revealed by permanganic etching, which can selectively etch the amorphous material of the interlamellar layers [36]. Figure 10 presents the SEM micrographs of the skin and core layers of the IM samples compressed along the t.d. to a true strain ranging from 0 to 0.8. The narrow micrographs presented in the first left column illustrate the initial morphology of the sample before deformation. These micrographs show the same morphology as already observed in Figure 2, just to recall the essential features of the morphology of the skin (upper row) and core (bottom row) layers. As was already discussed, the lamellae in the skin layer are well-oriented parallel to the t.d., while the preferred orientation of lamellae in the core layer is almost invisible. These lamellae in the core layer seem to be organized in higher-order structures, such as spherulites, which can be recognized at a lower magnification. The lamellae in the skin layer appear shorter than those in the core layer, although this look can be artificial, as has already been discussed earlier in this section. The micrographs of the sample deformed to a relatively low true strain of e = 0.4, which is within the strain range of a hump indicative of the second yield in the stressstrain curve, show some changes in the orientation of lamellae due to the active deformation mechanisms. In some areas (marked with highlighted circles on the micrographs), an early stage of the formation of lamellar kinks can be observed. These early kinks, which are not yet well developed, can be recognized in both the skin-and core structures. As illustrated by the micrographs of samples compressed to the true strain of e = 0.5 and e = 0.8, presented in the middle and on the right-hand side of Figure 10, the kinks become more mature and sharper as the strain increases. Moreover, the number of kinks that can be identified in each micrograph increases with the increasing strain, especially in the skin layer, which exhibits a well-oriented lamellar structure. This finding is reasonable because the number of lamellar stacks parallel to the direction of the load, which are the most susceptible to microbuckling and kinking, is significantly greater in a well-oriented skin layer than in the core layer, showing only a poor orientation. At e = 0.8, fairly well-developed and regular kinks can be easily seen in the skin layer, which locally lead to a chevron morphology. Now, virtually As discussed above, the mechanical and X-ray scattering data, presented in our previous papers [10,11,15] as well as in this article, strongly support the hypothesis of deformation instability in the form of the microbuckling of lamellae, followed by their kinking and the local formation of a chevron morphology. The microbuckling instability leading to sinusoidal undulations of the lamellae is initially elastic [16], but the subsequent formation of kinks entails some plastic deformation and possibly damage phenomena around the hinge of the kink [11,21]. This manifests itself macroscopically in the stress-strain curve in the form of a hump, commonly referred to as the second macroscopic yield, as the microbuckling helps to overcome the temporary barrier to further deformation and allows the relatively easy plastic deformation to continue, facilitating new deformation mechanisms in the just-kinked lamellae-such as crystallographic slips, previously inaccessible to these lamellae before buckling. However, to obtain the direct evidence of such postulated behavior of the material during its deformation, microscopic observations of deformed samples that could confirm conclusions drawn from the X-ray data seemed highly desirable. Therefore, the microscopic observations of samples deformed to various strains were carried out using a scanning electron microscope (SEM). Both the skin and core of the sample were examined in the CD-view (LD-FD observation plane). The LD-FD plane of observation was first exposed by microtoming, and then the lamellar morphology in this plane was revealed by permanganic etching, which can selectively etch the amorphous material of the interlamellar layers [36]. Figure 10 presents the SEM micrographs of the skin and core layers of the IM samples compressed along the t.d. to a true strain ranging from 0 to 0.8. The narrow micrographs presented in the first left column illustrate the initial morphology of the sample before deformation. These micrographs show the same morphology as already observed in Figure 2, just to recall the essential features of the morphology of the skin (upper row) and core (bottom row) layers. As was already discussed, the lamellae in the skin layer are well-oriented parallel to the t.d., while the preferred orientation of lamellae in the core layer is almost invisible. These lamellae in the core layer seem to be organized in higher-order structures, such as spherulites, which can be recognized at a lower magnification. The lamellae in the skin layer appear shorter than those in the core layer, although this look can be artificial, as has already been discussed earlier in this section. The micrographs of the sample deformed to a relatively low true strain of e = 0.4, which is within the strain range of a hump indicative of the second yield in the stress-strain curve, show some changes in the orientation of lamellae due to the active deformation mechanisms. In some areas (marked with highlighted circles on the micrographs), an early stage of the formation of lamellar kinks can be observed. These early kinks, which are not yet well developed, can be recognized in both the skin-and core structures. As illustrated by the micrographs of samples compressed to the true strain of e = 0.5 and e = 0.8, presented in the middle and on the right-hand side of Figure 10, the kinks become more mature and sharper as the strain increases. Moreover, the number of kinks that can be identified in each micrograph increases with the increasing strain, especially in the skin layer, which exhibits a well-oriented lamellar structure. This finding is reasonable because the number of lamellar stacks parallel to the direction of the load, which are the most susceptible to microbuckling and kinking, is significantly greater in a well-oriented skin layer than in the core layer, showing only a poor orientation. At e = 0.8, fairly well-developed and regular kinks can be easily seen in the skin layer, which locally lead to a chevron morphology. Now, virtually all the lamellae change their orientation from the initial, parallel to LD = t.d., to the inclined one. Lamellae inclined with respect to the LD experience a significantly higher resolved shear stress in potential slip systems than they do in the initial orientation parallel to LD, therefore crystallographic slip mechanisms can be easily activated in such lamellae, reoriented in kinks, to continue the deformation process [4,49,51]. The same phenomena also take place in the much less oriented core part of the sample, although here the kinks, which are much less numerous than in the oriented skin layer, can only locally support the main deformation mechanism-the crystallographic chain slip, which was activated earlier, at the yield point, in other lamellae already oriented favorably for the slip mechanism.
all the lamellae change their orientation from the initial, parallel to LD = t.d., to the inclined one. Lamellae inclined with respect to the LD experience a significantly higher resolved shear stress in potential slip systems than they do in the initial orientation parallel to LD, therefore crystallographic slip mechanisms can be easily activated in such lamellae, reoriented in kinks, to continue the deformation process [4,49,51]. The same phenomena also take place in the much less oriented core part of the sample, although here the kinks, which are much less numerous than in the oriented skin layer, can only locally support the main deformation mechanism-the crystallographic chain slip, which was activated earlier, at the yield point, in other lamellae already oriented favorably for the slip mechanism.
We believe that the presented micrographs, clearly showing the formation of lamellar kinks already at relatively low strains around e  0.4, provide convincing evidence of the microbuckling deformation instability, which in our opinion is the mechanism responsible for the second macroscopic yield that is frequently observed in semicrystalline polymers. Figure 10. SEM micrographs of the LD-FD plane of the IM samples deformed to the indicated true strains of 0, 0.4, 0.5, and 0.8 by the plane-strain compression parallel to the t.d. direction. The direction of compression is indicated by thick arrows on the right-hand side. Upper row: samples taken from the skin layer. Bottom row: samples taken from the core layer. Samples were etched with permanganic etchant before observations to reveal the lamellar morphology. Bright yellow circles highlight the lamellar kinks that were formed during deformation.

Conclusions
The study of the deformation of HDPE allowed concluding that the deformation process of a semicrystalline polymer depends not only on the common deformation mechanisms that are active in a broad range of strain, such as the crystallographic slip or interlamellar shear in amorphous layers. As already established, these basic mechanisms are occasionally supported by other specific mechanisms, such as twinning or martensitic transformation, when possible [1,2,4]. Furthermore, cavitation-the instability affecting primarily the amorphous phase-appeared important for the deformation of also the crystalline phase in certain deformation modes, such as uniaxial extension, and for the final structure and morphology of the deformed material. Our recent studies revealed, in turn, that some more subtle phenomena, like other deformation instabilities-e.g., microbuckling or Figure 10. SEM micrographs of the LD-FD plane of the IM samples deformed to the indicated true strains of 0, 0.4, 0.5, and 0.8 by the plane-strain compression parallel to the t.d. direction. The direction of compression is indicated by thick arrows on the right-hand side. Upper row: samples taken from the skin layer. Bottom row: samples taken from the core layer. Samples were etched with permanganic etchant before observations to reveal the lamellar morphology. Bright yellow circles highlight the lamellar kinks that were formed during deformation.
We believe that the presented micrographs, clearly showing the formation of lamellar kinks already at relatively low strains around e ≈ 0.4, provide convincing evidence of the microbuckling deformation instability, which in our opinion is the mechanism responsible for the second macroscopic yield that is frequently observed in semicrystalline polymers.

Conclusions
The study of the deformation of HDPE allowed concluding that the deformation process of a semicrystalline polymer depends not only on the common deformation mechanisms that are active in a broad range of strain, such as the crystallographic slip or interlamellar shear in amorphous layers. As already established, these basic mechanisms are occasionally supported by other specific mechanisms, such as twinning or martensitic transformation, when possible [1,2,4]. Furthermore, cavitation-the instability affecting primarily the amorphous phase-appeared important for the deformation of also the crystalline phase in certain deformation modes, such as uniaxial extension, and for the final structure and morphology of the deformed material. Our recent studies revealed, in turn, that some more subtle phenomena, like other deformation instabilities-e.g., microbuckling or lamellae fragmentation due to slip localization-may also play a very important role in the deformation sequence of a semicrystalline polymer [10,11,15]. These instabilities are often needed to modify the deformation sequence or enable the activation of new mechanisms in order to facilitate strain accommodation in a way that minimizes energy consumption and prevents the premature failure of the material.
In this work, the important role of the deformation instability through lamellae microbuckling was studied in linear polyethylene (HDPE), selected as a representative semicrystalline polymer. The microbuckling instability occurs early in HDPE at a relatively low true strain of around e = 0.3. It is experienced by lamellar stacks, which are specifically oriented parallel to the compression direction (actually, the same can happen in tensile deformation when the lamella stacks are drawn perpendicularly to layering). Microbuckling, initially elastic, quickly transforms with increasing strain into the cooperative folding of lamellae and the formation of angular kinks, involving non-reversible plastic deformation and/or limited damage, especially in the hinges of sharp kink profiles. Microbuckling, resulting in the formation of lamellar kinks and sometimes a chevron-like morphology, as evidenced by the X-ray and electron microscopic observations reported in this article, appears extremely important for the subsequent deformation behavior of a semicrystalline polymer, especially in some oriented structures, since kinking induces the rapid and practically irreversible rotation of these lamellae, which were oriented initially parallel to the compression (such as, e.g., those in polar regions of spherulites or in oriented skin layers of the injection-molded sample when compressed perpendicularly to the injection direction). Before buckling, these lamellae were not able to deform by any crystallographic mechanism due to the too low resolved shear stress in the plane and direction of potential slip; consequently, the deformation was temporarily locked locally in these areas. The reorientation of the lamellae in the kinks initiated by microbuckling results in an increase in the resolved shear stress for potential crystallographic slip systems. At a certain strain, this increase may appear sufficient to activate the slip mechanism and initiate then an extensive plastic deformation. This opens up a new deformation route of relatively easy plastic deformation-the kinked lamellae can now deform by crystallographic slip, like other lamellae that have already been oriented favorably for a crystallographic slip. This provides easier strain accommodation and precludes excessive stress build-up, thus preventing the premature failure of the material. This transition induced by microbuckling/kinking instability frequently manifests itself in the stress-strain curve as a broad hump, referred to as the second macroscopic yield.
Microbuckling/kinking instability, although appearing to be a common deformation mode that may operate in the deformation of materials of various structures and morphologies, can be particularly important in deforming well-oriented lamellar structures-e.g., in the drawing of the pre-oriented films of semicrystalline polymer, a process commonly used in many technologies, such as the production of porous membranes.